The Electromagnetic (EM) Inspection of Offshore Wire Ropes Herbert R. Weischedel NDT Technologies, Inc. P.O.Box 637, South Windsor, CT 06074, Tel. (860) 644-5655Introduction Because the reliable and safe use of wire rope is crucial for offshore applications, concern with their integrityis a constant preoccupation of wire rope operators and safety authorities. In spite of these concerns, a reluctanceto apply appropriate inspection methods and discard criteria compromises the safety of many offshore operations.A recent multi-hundred-million-dollar accident, caused by a wire rope failure, underscores the importance ofreliable wire rope inspection methods. Because many offshore ropes deteriorate internally without externally visible signs, their inspection solely byvisual methods is unsafe. In other cases, visual inspection is possible but not practical. For example, mooringropes are often covered with mud and marine growth. This makes their visual inspection difficult, if notimpossible. When visual inspections are impossible, rope operators usually resort to a statutory life policy as analternative. (The statutory life method requires rope retirement at prescribed, fixed intervals.) By definition, thisapproach must be extremely conservative and, therefore, wasteful. For example, presently, countless perfectlygood crane ropes - worth many millions of dollars - are discarded at regular annual intervals. And yet, in spite ofthis very uneconomical practice, occasional rope failures still occur. More dependable inspection methods, combined with a better understanding of degradation mechanisms and discard criteria, can notably increase wire rope safety. For example, Figure 1. Mooring rope inspection electromagnetic (EM) nondestructive inspections at regular intervals can significantly increase the safety of offshore ropes. EM inspections are particularly effective when they are combined with visual examinations and a thorough understanding of rope deterioration modes. Two different and distinct EM methods have evolved for the detection and measurement of rope defects • Loss of Metallic Cross-Sectional Area (LMA) Inspection, which (quantitatively) measures loss of metallic cross-sectional area caused by external or internal corrosion (due to environmental conditions or poor lubrication) and wear (due to rubbing along floors, nicking, high pressures, and/or poor lubrication). • Localized-Flaw (LF) Inspection, which (qualitatively) detects a wide variety of external and internal discontinuities such as broken wires and corrosion pitting. Broken wires are usually caused by fatigue, interstrand nicking and martensitic embrittlement. Modern dual-function EM rope testers allow simultaneous LMA and LF inspections. Figure 1 shows the EMinspection of an oil platform mooring rope.Underlying Principles For all present dual-function instruments, strong permanent magnets induce a magnetic flux at the saturationlevel in the rope in the axial (longitudinal) direction. Various types of sensors, such as coils, Hall sensors orfluxgate sensors close to the rope sense and measure the magnetic flux. Any discontinuity – such as a broken wire or corrosion pitting – distorts the magnetic flux in the rope andcauses it to leak from the rope. For LF inspections, the radial component of the leakage flux is measured by so-called radial sensors. Note that these sensors are also called differential sensors because they sense onlychanges of the magnetic flux in the rope and not the flux itself. Therefore, flaw detection depends on a rapidchange of the magnetic flux, which is typically caused by broken wires and corrosion pitting. Differential sensorscannot detect more gradual changes of the rope flux, which are typically caused by wear and corrosion.
Methods for the (quantitative) measurement of the LMA of a rope are discussed in the following. When arope is magnetically saturated, the axial magnetic flux in the rope is proportional to its cross-sectional area.Therefore, any LMA can be determined by measuring this magnetic flux. Two types of sensors can be used tomeasure magnetic flux: Hall sensors (or, alternatively, fluxgate sensors) and coils in combination with electronicintegrator circuits. To measure flux density, Hall sensors (and fluxgate sensors) must be physically inserted directly into themagnetic flux path. Thus, the flux to be measured must intersect the sensors. This is not possible whenmeasuring the magnetic flux inside the rope. Therefore, instruments that use Hall sensors or fluxgate sensorsmust always resort to an indirect method for determining the axial rope flux. They measure some flux densityoutside the rope and determine or estimate the longitudinal rope flux from the external flux measurement.Alternatively coils-cum-integrators can be used. Because coils must encircle the magnetic flux to be measured,they can directly measure the magnetic flux inside the rope. Currently, two generic methods are used for thedetermination of LMA. They are illustrated in Figure 2. The Main-Flux Method uses an annular coil together with an electronic integrator circuit to determine thelocal magnetic flux inside the rope (Figure 2a). Note that the coil must encircle the rope. Originally patented1 inBritain in the 1960s, this approach has been discussed in the literature.2, 3, 4 Since it measures the magnetic fluxinside the rope locally, the annular coil approach offers uncommon resolving power, signal fidelity and, therefore,inspection accuracy. The performance of this arrangement is unsurpassed and must be considered the GoldStandard by which all other methods are measured. FIGURE 2. Cross-sectional area measurement methods Return Flux Path Annular Coil (cum Integrator) Sense Coils (cum Integrator) Yoke Permanent Magnet External Rope Stray Flux Path External Stray Flux Path Main Flux Path Integrator Integrator a. Main-Flux Method b. Modified Main-Flux Method Flux Gate Sensors Hall Sensors c. Return-Flux Method d. Return-Flux Method Unfortunately, it is topologically impossible to implement a hinged annular coil with a large number of turnsthat can be opened and conveniently attached to the rope. This means, the practical implementation of the main-flux method for in-service wire rope inspections is seriously hampered by an inherent and insurmountableproblem: An annular coil – encircling the rope – must be wound onto the rope in the field for each inspection. This
cumbersome procedure allows only very few turns (say, one hundred) and, hence, only very small induced coilvoltages. The coil voltages are of the same order of magnitude as the always-present offset voltages at the inputof operational amplifiers that are used for the design of electronic integrator circuits. These inherent offsetvoltages make the long-term low-drift integration of the coil voltages impossible. Hence, the annular coil approachis not feasible for in-service inspections where LMA measurements over longer time periods – say, over morethan a few minutes – are required. The Modified Main-Flux Method, shown in Figure 2b, tries to retain the superior performance of the Main-Flux Method while allowing the implementation of hinged sense heads of the clamshell design.3, 4 The test signals of this Modified Main-Flux Method are a combination of the Main-Flux signal and a signalcomponent that is caused by the (parasitic) outside stray flux, i.e., that portion of the flux that leaves and entersthe sense head to and from the outside, respectively, and flows along some external stray flux path (seeFigure 2). Unfortunately, this outside signal component is significant. It compromises the quality of the test resultsand must be considered parasitic. Although this parasitic effect can be minimized,5 a true signal of the main fluxtype cannot be completely restored. Nevertheless, the Modified Main-Flux Method retains at least some of thedesirable features of the annular coil approach. The Return Flux Method uses Hall sensors6, 7 (or, more complex, fluxgate sensors8) to measure themagnetic flux in the magnetic return path of the instrument. Illustrated by Figures 2c and d, the return flux isequal to the average value of the axial rope flux inside the sense head plus the outside stray flux. Therefore, thereturn flux provides an estimate of the average cross sectional area of that section of the rope that is inside thesense head. Flux sensors can either be inserted into the air gap between the permanent magnet poles and therope or into the yoke of the magnetizer assembly. The return-flux method allows the design of hinged sensorheads of the clamshell type. This feature makes it possible to attach the sensor head to the rope even underadverse field conditions.Signal Generation and Evaluation5 For the interpretation of test results and for a correlation of test data with the actual rope condition, the ropeinspector must understand the capabilities and limitations of his EM rope inspection equipment. A properappreciation of the signal generation process, together with an understanding of rope degradation mechanismsand discard criteria, is essential for making rational rope retirement decisions. For the following discussion, step changes of metallic cross-sectional area – caused by missing or addedwires, for example – have particular significance. Because of its simple geometry, a step change can be called afundamental defect. Accordingly, the corresponding LMA and LF signals, caused by a fundamental defect, can be called fundamental LMA or LFFIGURE 3. Input and output signals of an idealized rope test instrument signals, respectively. The Distance on Rope fundamental signals can also be called an instrument’s step Decreasing Gap Widths response. It is easy to see that any defect can be represented as the Rope Cross-Section sum of appropriately scaled and spaced fundamental defects. 0 Moreover, the process of signal generation is, at least LMA Trace (ideal) approximately, linear. Hence linear superposition applies. 0 This means that, if a defect can be represented as the sum of several fundamental defects, LF Trace then the corresponding defect 0 (LMA and LF) signals are the sum of the corresponding Alternative LF Trace fundamental LMA and LF signals. The concepts of fundamental defects and signals, step response, and linear
superposition are discussed further in the literature.9 Determining and evaluating its step response is an excellentmethod for characterizing the performance of an EM wire rope tester. In the present context, the concept of filtering can be used very loosely. For example, the sensor head of anEM rope tester, together with the signal electronics, may be viewed as a – linear or nonlinear – data filter. This isillustrated further by Figure 3. The figure depicts the rope cross-section as the input signal and the idealizedcorresponding LMA and LF output signals. Note that, for many rope testers, the LF signal approximates the firstderivative of the rope cross-section signal. For other instruments, the LF signal is the second derivative of therope cross-section, as shown as Alternative LF Signal in Figure 3. Note that the signals generated with the MainFlux Method, shown in Figure 2a, closely resemble the idealized results of Figure 3. Recognizing differentiation as the quintessential high-pass filter operation, the LF signal can be consideredas the rope cross-section input signal that has been high-pass filtered. High-pass filtering accentuates fastchanges of signals, and, typically, broken wires and corrosion pitting cause rapid variations of the rope cross-section. Therefore, the high-pass filtering feature makes the LF Signal useful for the detection of broken wiresand corrosion pitting. Any inspection equipment should present data in a form that facilitates their interpretation by the humanoperator. Figure 3 shows that a perfect LMA signal could serve as such an accurate and conceptually simplemap of a rope’s LMA that is easy to interpret by the inspector.Resolution and Averaging Length The dictionary defines resolution as “the level of detail that can be distinguished in an image (or arecording).” For electromagnetic wire rope inspections, resolution is always the premier performance measure.In nondestructive testing, the terms resolution and inspection accuracy are often used synonymously.In the discipline of electromagnetic wire rope inspection, quantitative resolution3 or averaging length (sometimesalso called scanning length) is defined as the minimum length of a uniform anomaly for which the sensor providesan accurate measurement of a rope’s LMA. To visualize the concept of averaging length, assume that, instead of measuring metallic cross-sectionalarea directly, the rope tester continuously measures the metallic volume of consecutive rope sections with lengthsthat are equal to its averaging length. Figure 4 illustrates this concept. Figure 4a shows a FIGURE 4. LMA length and averaging length (hypothetical) rope with a LMA Length uniform 10% LMA extending 300 mm LMA Length 300 mm over a length of 300 mm. An instrument with a 50 mm averaging length will correctly 10% LMA 10% LMA measure this LMA. As illustrated by Figure 4b, a rope tester with an averaging Averaging Length Averaging Length length of 300 mm will also 50 mm 300 mm give a true indication of this a. b. anomaly. Now consider a LMA LMA (hypothetical) rope with a 10% Length 50 mm Length 50 mm uniform LMA extending over a length of 50 mm. Figure 4c shows that an instrument with 10% LMA 10% LMA an averaging length of 50 mm can determine the exact LMA caused by this anomaly. Averaging Averaging Length However, as can be seen Length 50 mm 300 mm from Figure 4d, an instrument c. d. with a an averaging length of 300 mm would indicate thesame anomaly as a 1.7% LMA extending over a length of 300 mm – a very inaccurate indication of the true ropecondition. These examples show the importance of a short averaging length.
Note that signal FIGURE 5. LMA signals as a function of averaging length averaging is a Decreasing Gap Width quintessential type of low- pass filtering, and that Rope Cross-Section signals lose a significant amount of information (details) by low-pass Increasing Averaging Length filtering. Figure 5 0 illustrates this situation. It shows how the quality of LMA signals deteriorates LMA Signals LMA Signals 0 as the averaging length increases. An analogy can illustrate the problems 0 associated with long LMA averaging lengths: A chain LMA Signals is only as strong as its 0 weakest link. Obviously, the strength of a chain is not determined by the average strength of some of its links. Similarly, thestrength of a rope, which has lost metallic cross-section by corrosion and/or wear, is determined by the minimumlocal metallic cross-sectional area along the rope’s length, and not by some average value of the rope cross-sectional area. Experience has shown that serious rope deterioration can occur over very short distances along the lengthof a rope. Hence, in order to determine and evaluate a rope’s actual metal loss with acceptable accuracy, a shortaveraging length – of no more than a few centimeters – is important. Because all wire rope testers have a quantitative resolution or averaging length that is greater than zero, anaccurate measurement of LMA always requires minimum lengths of anomalies. As the above discussion showsand as illustrated by Figure 5, the concept of quantitative resolution or averaging length is important for specifyingand comparing the performance of rope testers.Wire Rope Inspection and Retirement Two different philosophies have been used to effect rope retirement:1. A Statutory Life Policy mandates rope retirement at certain prescribed intervals.2. Retirement for Cause is based on retirement conditions that are evaluated periodically by nondestructive inspections. Because a Statutory Life Policy is inherently wasteful, regulators have tended to adopt the Retirement-for-Cause approach wherever appropriate. Wire rope deteriorates gradually throughout its entire service life. To keep abreast of deterioration, wire ropemust be periodically inspected. Because moderate deterioration is normally present, the mere detection of ropedeterioration does not usually justify rope retirement. There are two major nondestructive inspection methods forthe detection and evaluation of rope degradation: Visual inspections and EM inspections.Visual Inspection Visual inspections are a simple yet useful method for detecting a wide variety of external rope deteriorations.Using this approach, the rope is moved two or three feet at a time and visually examined for broken wires andother rope deterioration at each stop. This method is tedious and, because the rope is often covered with grease,many external and internal defects elude detection. Another visual inspection tool is measurement of the rope diameter. Rope diameter measurements comparethe original diameter – when new and subjected to a known load – with the current reading under likecircumstances. A change in rope diameter indicates external and/or internal rope damage. Inevitably, many sortsof damage do not cause a change of rope diameter.
Visual inspections are inherently not well suited for the detection of internal rope deterioration. Therefore, theyhave limited value as a sole means of wire rope inspection. However, visual inspections are simple and do notrequire special instrumentation. When combined with the knowledge of an experienced rope examiner, visualinspection can provide a valuable supplementary tool for evaluating many forms of rope degradation.Electromagnetic Inspections " As discussed, EM wire rope inspection gives detailed insight into the condition of a rope. Its reliability has "made EM testing a universally accepted method for the inspection of wire ropes in mining, for ski lifts, and manyother applications.Combined Inspections Electromagnetic and visual wire rope inspections complement each other. Both are essential for safe ropeoperation, and both methods should therefore be used for maximum safety. A thorough inspection must consider all aspects of a ropes condition, including:1. The findings of a visual inspection,2. the results of an EM rope inspection,3. the ropes operating conditions and related damage mechanisms,4. the history of the rope under test and that of its predecessors. Dependable inspection procedures, using combined visual and EM methods, can detect rope deterioration atits earliest stages. Therefore, wire rope users can employ them as an effective preventive maintenance tool. Toillustrate, here are some practical examples.1. The early detection of corrosion allows immediate corrective action through improved lubrication.2. Accelerating wear and interstrand nicking can indicate a need to reline sheaves to stop further degradation3. Careful inspections can monitor the development of local damage at the crossover points of the rope on a winch drum. This way, the operator can determine the optimum time for repositioning the rope on the drum. A program of periodic inspections is especially effective. To establish baseline data for subsequentinspections, such a program should commence with an initial inspection of the installed rope after a certain break-in period. Subsequent inspections should then be performed at scheduled intervals. In particular, periodic EMinspections allow the documentation of a ropes deterioration over its entire service life.Offshore Ropes10, 11 Many offshore crane and diving bell ropes are of the torque-balanced multistrand type comprising two ormore layers of strands. Figure 6 shows a cutaway section of such a multistrand rope. Torque balance is achievedby laying outer and inner strands in opposite directions. This type of rope construction limits axial rotation of thefreely suspended rope under load. In addition, multistrand ropes offer flexibility and a wear resistant surfaceprofile. FIGURE 6. Multistrand FIGURE 7. FIGURE 8. Broken wires in Rope construction Interstrand nicking second layer of strands Wire in Second Layer of Strands Interstrand Nicking and Wear at Wire Crossovers Wire in First Layer of Strands However, the wires and strands in different layers of these ropes touch locally and at an angle. Therefore,when multistrand ropes bend over sheaves or on a drum, they are subject to the combined effect of radial loading,
relative motion between wires and bending stresses. This causes fretting wear or fatigue and interwire nickingacross the interface between layers as illustrated by Figure 7. Therefore, multistrand ropes are prone to develop internal broken wires. This breakup occurs primarily on theinterface between the outer and second layer of strands, usually with no externally visible signs (see Figure 8).The wires in the second layer of strands typically show interstrand nicking and breaks caused by a combination offluctuating axial wire stresses, inter-wire motions and fluctuating radial loads. The broken wires usually showsquared-off and z-shaped ends that are typical for fatigue breaks. Many multistrand ropes are subject to corrosive FIGURE 9. Two sections of crane rope environmental conditions. For example, offshore ropes are with severe internal corrosion either immersed in the sea or continually wetted by salt water spray. In addition, heavy use in a marine environment can displace and degrade the rope lubricant. The combined effects of fatigue, corrosion and lubricant degradation can cause rapid internal deterioration where there is no effective form of protection. The combined effects of fatigue, corrosion, and lubricant degradation can cause fairly rapid internal degradation with no externally visible indications. Figure 9 illustrates this situation. The upper part of the figure shows the external appearance of an offshore crane rope; the lower part is another section of same rope with the outer strands stripped away. While itwould be straightforward to detect this type of rope deterioration with an EM inspection, this situation is by nomeans unique and has caused several in-service rope failures.Example 1. Diving bell rope inspection. FIGURE 10. Chart of diving bell hoist rope 60 65 70 Distance (m) LMA Trace LF Trace Figure 10 shows an EM inspection chart recording of a 30 mm die-formed multistrand diving bell hoist rope.The rope shows periodic groups of broken wires, probably at cross-over points on the winch drum. The maximumLMA is 1%. The external broken wires could be identified visually. This rope section is subjected to the full in-airweight as the bell is lowered and raised. On the basis of the EM inspection, a decision was made to cut andreterminate the rope behind the first defect about 58 m from the diving bell.Example 2. Experimental multistrand rope inspection This case study illustrates the use of EM wire rope inspections for the detection and quantitativecharacterization of internal broken wires and clusters of broken wires in multistrand ropes. The presentexperiment deals with the inspection of a torque balanced multistrand rope with no corrosion and many internalbroken wires. This rope has been used on a trial basis and was known to contain numerous internal broken wiresalong its entire length. The task at hand was to determine the number of broken wires in 100 mm segments along the length of therope. The difficulty of this quantitative defect characterization problem was compounded by the fact that anundamaged rope section was not available for comparison. Further, at the time, the correlation of the typicaldeterioration modes of this and similar ropes with their EM inspection results was generally not well understood. A cross-sectional diagram of this multistrand rope is shown in Figure 11. As indicated in the figure, it is knownthat broken wires in multistrand ropes usually develop in the second layer at the interface between the first and
the second layer of strands. In addition, from this and similar ropes’ service histories, it can be assumed that therope under inspection has developed significant interstrand nicking together with numerous fatigue breaks ofwires in the second layer of strands. FIGURE 11. Typical position of The detailed detection and quantitative characterization of internalbroken wires in a multistrand rope broken wires in ropes with many breaks and clusters of breaks – such as the present rope – pose problems. Difficulties are caused by the fact Typical Positions that, for electromagnetic wire rope inspections, the indication of a broken of Broken Wires wire is influenced by a number of parameters like a) broken wire cross-sectional area, b) broken wire gap width, and c) by the position of the broken wire within the cross-section of the rope. d) For clusters of broken wires, an additional problem is caused by the fact that the relative position of broken wires with respect to each other along the length of the rope is not known. For example, the gaps of broken wires could be aligned or staggered. e) Finally and most importantly, broken wires with zero or tight gap widths are not detectable by electromagnetic inspections because they do not produce a sufficient magnetic leakage flux. Considering the above, only an estimate of the number of broken wires is possible. Conventionally, the LF trace is used FIGURE 12. LMA and LF traces and for the detection of broken wires. relative number of broken wires However, the LF signal is not quantitative Distance (meter from marker) and can not be used for estimating the -5 -4 -3 -2 -1 0 1 2 1 5 number of broken wires. On the other Relative Number of Broken Wires (N/Nmax) hand, the LMA trace of the inspection N/Nm ax 4 chart in Figure 12 shows rapid relatively small variations of cross-section. These 0 3 variations are significant and can be used to estimate the number of broken wires Change of Cross-Section(%) per unit of rope length. Note, however, High-Pass Filtered 2 that the averaging length or quantitative resolution of the instrumentation used -1 1 must be sufficient to allow this quantitative defect characterization. 0 The estimated number of broken LF wires per 100 mm of rope length, N, -2 -1 derived from the LMA trace, is shown on the top of Chart 12. Here, Nmax denotes the maximum number of broken wires per100 mm of rope length. Based on the operating history of this and similar ropes, a value of Nmax = 20 can beestimated. The rope was subsequently disassembled12 to determine the actual number of broken wires per unit of ropelength. Broken wire estimates together with the actual number of broken wires along the length of the rope areshown in Figure 13. Considering the fact that the LMA trace not only indicates broken wires but also interstrandnicking, internal wear and other disturbances of the rope structure, there is a good correlation between the actualand estimated number of internal broken wires. The correlation between actual and estimated number of brokenwires up to a rope distance of about 4500 mm is very good. Beyond this distance, there is an offset, which isprobably due to a distance measurement error during disassembly of the rope. A destructive break test of the rope showed a 30.2% loss of breaking strength. On the other hand, thesecond layer of strands of the rope (see Figure 11) represents about 30% of the total rope cross-sectional area.This leads to the hypothesis that, for this rope, the second layer of strands has lost all load-bearing capability. The lack of sufficient information on the rope’s operating history – and that of its predecessors – made thisrope evaluation difficult. Under normal circumstances, these details are known and must be considered whenassessing the rope condition. Altogether, this evaluation shows that a quantitative defect characterization for
ropes with internal broken wires and clusters of broken wires is possible. The example illustrates the capabilities and limitations of EM wire rope inspection methods for this particular defect characterization problem. FIGURE 13. Broken wires at 100 mm intervals (smoothed data, 3 sample average) FIGURE 14. Typical Broken Wires at 100 mm Intervals 6 strand independent (Smoothed Data, 3 Sample Average) 14 wire rope core (IWRC) rope 12Number of Broken Wires per 100 mm Interval 10 8 6 4 2 Actual Estimate IWRC 0 0 00 00 00 00 00 00 00 00 00 00 00 00 00 00 00 0 50 10 15 20 25 30 35 40 45 50 55 60 65 70 75 80 Distance on Rope (mm) Example 3. Mooring rope inspection This example deals with the inspection of an IWRC (Independent Wire Rope Core) mooring rope with a diameter of 89 mm whose inspection is depicted in Figure 1. Figure 14 shows a typical cross-sectional diagram of such a rope. For IWRC ropes, the outer wires of the outer strands have a larger diameter than the outer core strand wires. To minimize interstrand nicking between the outer strands and the IWRC, these ropes are designed such that the wires of the outer strands and the IWRC are approximately parallel. (This is usually achieved by choosing a lang lay construction for the IWRC and an ordinary lay construction for the outer strands.13) Typically, the wires of the outer strands are well supported by their neighbors while the outer wires of the IWRC are relatively unsupported. The result of these geometrical features is that, under fluctuating tensile loads, the outer IWRC wires are continuously forced into the valleys between the outer strand wires and then released. This mechanism results in secondary bending stresses in the core wires leading to large numbers of fatigue breaks. These breaks can be very close together and can form groups of breaks. Eventually, the IWRC can completely disintegrate into short pieces of wire about half a lay length long. FIGURE 15. Inspection chart of 89 mm IWRC mooring rope 18. with corrosion and severe core damage LMA Trace LF Trace Figure 15 shows the results of the present mooring rope inspection. The chart recording indicates a severe breakup of the independent wire rope core, which is strong evidence of heavy fluctuating tensile fatigue loading. Note that the LMA and LF traces show the typical patterns of broken and missing wires (see Figure 3). The missing wire patterns indicate that short pieces of broken IWRC wires might have fallen out of the rope. In addition, together with the findings of a visual inspection, the chart indicates severe corrosion, including corrosion pitting. Note that corrosion products are clearly visible in Figure 1.
Summary and Conclusions For most offshore ropes, inspection solely by visual methods is either unsafe or not practical. On the otherhand, electromagnetic (EM) inspections at regular intervals can significantly increase confidence in the integrity ofoffshore ropes. Similar to other industries, the offshore oil and gas industry could derive considerable benefitsfrom EM inspections. EM inspections are particularly effective when they are combined with visual examinations as part of acomprehensive inspection program. For a thorough inspection, all aspects of a rope’s condition must beconsidered, including 1. the findings of a visual inspection, 2. the results of an EM rope inspection, 3. the rope’s operating conditions and damage mechanisms, 4. the history of the rope under test and that of its predecessors. A program of periodic inspections is especially effective. In particular, periodic EM inspections allow thedocumentation of a rope’s deterioration over its entire service life.Acknowledgment. The author wants to thank Professor Richard Chaplin from The University of Reading,England for many interesting discussions and suggestions.References1. Whitehead, E.A.N. “Method of Obtaining an Electrical Signal Proportional to the Cross-Sectional Area of a Magnetic Tube or Rod,” UK Patent 913,780 (December 1962).2. Rieger, W. “Ein Beitrag zur magnetinductiven Querschnittsmessung von Drahtseilen” (“A Contribution to the Magnet-Inductive Cross-Sectional Area Measurement of Wire Ropes”), Doctoral Dissertation, Universität Stuttgart, Germany (1983).3. Weischedel, H.R. “The Inspection of Wire Ropes in Service, A Critical Review.” Materials Evaluation. Vol. 43, No.13. American Society for Nondestructive Testing, pp. 1592-1605.4. Weischedel, H.R. “Method and Apparatus for Magnetically Inspecting Elongated Objects for Structural Defects.” US Patent 4,659,991 (April 1987).5. Weischedel, H.R. “Electromagnetic Wire Rope Inspection: Signal Generation, Filtering, and Computer-Aided Rope Evaluation.” Presented at The Nondestructive Testing of Rope. Krakow, Poland: (O.I.P.E.E.C.) International Organization for the Study of the Endurance of Wire Rope. (September 1999)6. Kitzinger, F. and G.A. Wint. “Magnetic Testing Device for Detecting Loss of Metallic Area and Internal and External Defects in Elongated Objects.” US Patent 4,096,437 (June 1978).7. Marchent, B.G. “Apparatus for Nondestructive Testing of Elongate Objects.” UK Patent Application GB 2 012 966 (December 1978).8. Tomaiuolo, F.G. and J.G. Lang. “Method and Apparatus for Nondestructive Testing of Magnetically Permeable Bodies Using a First Flux to Saturate the Body and a Second Flux Opposing the First Flux to Produce a Measurable Flux.” US Patent 4,495,465 (January 1985)9. Weischedel, H.R. “Quantitative In-Service Inspection of Wire Ropes, Applications and Theory.” International Advances in Nondestructive Testing, Vol. 15, New York: Gordon and Breach Science Publishers (1990): p. 83 – 118.10. Weischedel, H.R. and C.R. Chaplin. “Inspection of Wire Ropes for Offshore Applications.” Materials Evaluation. Vol. 49, No. 3. The American Society for Nondestructive Testing (1991): p. 362-367.11. Weischedel, H.R. and C.R. Chaplin. “The Inspection of Offshore Wire Ropes: The State of the Art.” Paper OTC 6969. Presented at Offshore Technology Conference. Houston, TX: (May 1992).12. Dohm. M. An evaluation of international and local magnetic rope testing instrument defect detection capabilities and resolution, particularly in respect to low rotation, multilayer rope constructions. Project Number GAP 503 and GAP 353. Johannesburg, South Africa: Safety in Mines Research Advisory Committee (1999).13. Wire Rope Users Manual, Third Edition. Woodstock, MD: Wire Rope Technical Board (1993).